O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a navegar o site, você aceita o uso de cookies. Leia nosso Contrato do Usuário e nossa Política de Privacidade.
O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a utilizar o site, você aceita o uso de cookies. Leia nossa Política de Privacidade e nosso Contrato do Usuário para obter mais detalhes.
Plant extracts are low-cost and biodegradable, and so the study
of plant extracts as corrosion inhibitors is an important
scientific research field due to both economic and
environmental benefits, our laboratory adopted a strategy of
evaluation of these molecules against corrosion of mild steel
in acid media. Many plant extracts have been used as effective
corrosion inhibitors of iron or steel in acidic media (El ouadi et
al., 2014; El Ouadi, ?; EL Ouadi et al., 2015; Manssouri et al.,
2015; El Mounsi et al., 2015; El Ouadi et al., 2015; Znini et
al., 2011; Elmsellem et al., 2014; Elmsellem et al., 2015;
Elmsellem et al., 2014; Elmsellem et al., 2013; Elmsellem et
al., 2015; Elmsellem et al., 2014; Aouniti et al., 2015;
Elmsellem et al., 2015). In this paper, electrochemical
polarisation, EIS and gravimetric techniques are applied to
study the ability of essential oil of Thymus Capitatus to inhibit
the corrosion of steel in 1M HCl. The effect of temperature is
Thymus Capitatus was harvested from "bosakour"(national
park) located in the area of Al-Hoceima (MOROCCO). The
harvest was in May 2010. The flowers, freshly harvested, are
dried in the shade in a dry, ventilated place for about 10 days.
Become dry, they are collected into clean bags for later use in
the extraction of essential oil.
Hydrodistillationapparatus and procedure
Often the hydrodistillation was performed by use of Deryng
apparatus or Clevenger type apparatus. In this extraction of
essential oil of the aerial part of Thymus Capitatus was
conducted by hydrodistillation using a Clevenger type
apparatus (Figure 1). The essential oil yields were measured.
Subsequently, received essential oils were dried over
anhydrous sodium sulfate and stored at 277 K in the darkness
before analysis, until gas chromatographic determination of its
Figure 1. Hydrodistillation by Clevenger apparatus
Essential oil isolation of Thymus Capitatus
The dried vegetal material (100 g) were water-distillated (3h)
using a Clevenger-type apparatus according to the method
recommended by the European Pharmacopoeia (Joulain and
König, 1998). The yield of fruits essential oil was 0.5%.
GC analysis were carried out using a Perkin-Elmer Auto-
system XL GC apparatus equipped with dual flame ionization
detection (FID) system and fused-silica capillary columns (60
m x 0.22 mmI.D., film thickness 0.25 μm), Rtx-1
(polydimethylsiloxane) and Rtx-wax (polyethyleneglycol).
The oven temperature was programmed from 60°C to 230°C
at 2°C/min and then held isothermally at 230°C for 35 min.
Injector and detector temperature was maintained at 280°C.
Samples were injected in the split mode (1/50), using helium
as carrier gas (1 ml/min); the injection volume was 0.2 μL of
pure oil. Component relative concentrations were calculated
based on GC peak areas without using correction factors.
Samples were also analysed using a Perkin-Elmer Turbo mass
detector (quadrupole), coupled to a Perkin-Elmer Auto-system
XL, equipped with fused-silica capillary columns Rtx-1 and
Rtx-Wax. Carrier gas: helium (1 mL/min), ion source
temperature: 150°C, oven temperature programmed from 60°C
to 230°C at 2°C/min and then held isothermally at 230°C (35
min), injector temperature: 280°C, energy ionization: 70 eV,
electron ionization mass spectra were acquired over the mass
range 35-350 Da, split: 1/80, injection volume: 0.2 μL of pure
Identification of components
The methodology carried out for identification of individual
components was based on: i) comparison of calculated
retention indices (RI), on polar and apolar columns, with those
of authentic compounds or literature data (Hochmuth et al.,
2001); ii) computer matching with commercial mass spectral
libraries (Adams, 2004) and comparison of mass spectra with
those of our own library of authentic compounds or literature
data (Hochmuth et al., 2001; Belfilali et al., 2014).
MATERIALS AND METHODS
Tests were performed on a cold rolled steel (CRS) of the
following composition (0.09%P; 0.38% Si; 0.01% Al; 0.05%
Mn; 0.21% C; 0.05% S and the remainder iron) were polished
with emery paper up to 1200 grade, washed thoroughly with
double-distilled water, degreased with A Rgrade ethanol,
acetone and dried at room temperature. MS samples of size 1.0
x 1.0x 1.0 cm and MS powder were used for weight loss
studies. For electrochemical studies, specimens with an
exposed area of 1 cm2
were used. These specimens were
degreased ultrasonically with 2-propanol andpolished
mechanically with different grades of emery paper to obtain
very smooth surface.
Preparation of solutions
The test solutions were prepared by the dilution of analytical
grade 37% HCl with distilled water up to the optimum
inhibitor concentration. For pH studies, the test solutions were
prepared by the dilution of distilled water up to the optimum
concentration where it can reach by adjusting the pH using
HCl and NaOH.
6868 El Ouadi et al. The use of essential oil of Thymus capitatus originating from North-East Morocco, as eco-friendly corrosion inhibitors
of mild steel in hydrochloric acid solution
Inhibitor was dissolved in acid solution at required
concentrations in (mL/L) and the solution in the absence of
inhibitor was taken as blank for comparison purposes. The test
solutions were freshly prepared before each experiment by
adding Thymus Capitatus oil directly to the corrosive solution.
Experiments were conducted on several occasions to ensure
reproducibility. Concentrations of Thymus Capitatus oil were
1.25, 2.5 and 5 mL/L.
Weight loss measurements
The weight loss is employed as the principal measure of
corrosion. Use of weight loss as a measure of corrosion
requires making the assumption that all weight loss has been
due to generalized corrosion and not localized pitting.
Although these tests are simple, there is no simple way to
extrapolate the results to predict the life time of the system
under investigation. Moreover, some corrosion processes
occur with no significant mass change (e.g. pitting corrosion)
making them difficult to detect by gravimetric method
(Chetouani et al., 2006; Kharchouf, 2011). The simplest way
of measuring the corrosion rate of a metal is to expose the
sample to the test medium (e.g. sea water) and measure the
loss of weight of the material as a function of time. The
gravimetric test is based on the immersion of the steel plates in
iron, in 100 ml of a 1M HCl solution containing the inhibitor
(Thymus Capitatus oil) at different concentrations, after be
Figure 2. Cathodic and Anodic polarisation curves of mild steel in 1M HCl in the
presence of essential oil of thymus capitatus at different concentrations
Figure 3. Nyquist plots in absence and presence of different concentrations of thymus
capitatus oil in HCL 1M
Figure 4. Variation of W in 1M HCl on steel surface without and with of optimum
concentration of thymus capitatus oil at different temperatures
6869 International Journal of Development Research, Vol. 06, Issue, 02, pp.6867-6874, February, 2016
degreased, polished and weighed. Immersion is subjected to a
temperature of 308 ° K to 6 hours. Temperature corrosive
environment is a factor that can affect the efficacy of
inhibiting it. Given the importance of this factor, we
performed tests of mass loss of steel in 1 M HCl with and
without addition of the inhibitor (Thymus Capitatus oil) at
different temperatures between 313 and 343 K.
As mentioned in the previous application notes, most
corrosion phenomena are of electrochemical nature and consist
of reactions on the surface of the corroding metal. Therefore
electrochemical tests methods can be used to characterize
corrosion mechanisms and predict corrosion rates. The
electrochemical measurements were performed using a
potentiostat PGZ100 piloted by Voltamaster soft-ware. This
potentiostat is connected to a cell with three electrode
thermostats with double wall (Tacussel Standard CEC/TH).
A saturated calomel electrode (SCE) and platinum electrode
were used as reference and auxiliary electrodes, respectively.
The working electrode (WE) in the form of disc was cut from
pure iron and was embedded in poly-tetra-fluoro-ethylene
(PTFE) to avoid any infiltration of electrolyte then exposing
only 1 cm2
surface to the aggressive solution. The test solution
was thermostatically controlled at 37 °C in air atmosphere
without bubbling. All potentials were measured against SCE.
The test solution was deaerated for 30 min at Ecorr in the cell
with pure nitrogen. Gas pebbling was maintained through the
experiments. Before recording the cathodic polarisation
curves, the iron electrode was polarized at 800 mV / SCE for
The potentiodynamic current–potential curves were recorded
by changing the electrode potential automatically from -800 to
-200 mV at a scanning rate of 1 mVs 1
, which are used for the
determination of corrosion current by the extrapolation of
anodic and cathodic Tafel lines to a point which gives log icorr
and the corresponding corrosion potential (Ecorr) for each
concentration of inhibitors and for the blank solution. The
electrochemical impedance spectroscopy (EIS) measurements
are carried out with the electrochemical system (Tacussel),
which included a digital potentiostat model Voltalab PGZ100
computer at Ecorr after immersion in solution without bubbling.
After the determination of steady-state current at a corrosion
potential, sine wave voltage (10 mV) peak to peak, at
frequencies between 100 kHz and 10 mHz are superimposed
on the restpotential. Computer programs automatically
controlled the measurements performed at rest potentials after
0.5 hour of exposure at 298 K. The impedance diagrams are
given in the Nyquist representation. Experiments are repeated
three times to ensure the reproducibility.
RESULTANTS AND DISCUSSION
Essential oil composition
Qualitative and quantitative analyses essential oils were done
using GC/MS analyses. The composition of essential oil of
Thymus Capitatus was shown in the Table 1.
Effect of concentration
Polarization study has been carried out in order to gain
knowledge about the kinetics of the anodic and cathodic
Figure 5. Arrhenius plots of lnW vs. 1000/T for mild steel in 1M HClin the absence and
the presence of oil thymus capitatus at optimum concentration (5 mL/L)
Figure 5’. The variation of Ln W / T vs 1000 / T of the steel in 1M HCl with and withoutoil of
thymus capitatus at optimum concentration (5 mL/L)
6870 El Ouadi et al. The use of essential oil of Thymus capitatus originating from North-East Morocco, as eco-friendly corrosion inhibitors
of mild steel in hydrochloric acid solution
reactions. Potentiodynamic curves are obtained in the presence
and the absence of the studied inhibitor, after pre-polarizing
the electrode at its Ecorr for 30 min, there after pre-polarized at
-800 mV for 10 min. After thisscan, the potential was swept
stepwise from the most cathodic potential to the anodic
direction. Potentiodynamic polarisation curves of steel in 1M
HCl in the presence and the absence of essential oil of thymus
capitatus is shown in Figure 2. The corrosion parameters
including corrosion current densities (Icorr), potential (Ecorr),
cathodic and anodic Tafel slope (βc and βa) and inhibition
efficiency (EI %) are listed in Table 2. In this case, the
inhibition efficiency is defined as follows:
Where I°corr and Icorr are, respectively the uninhibited and
inhibited current density respectively. The corrosion current
density was calculated from the intersection of cathodic and
anodic Tafel lines.
As it can be seen from Table 2, the Ecorr values were shifted
slightly toward the negative in the presence of the inhibitor in
comparison to that in it absence and the values of corrosion
potential nearly remain constant with the addition of different
concentration. These results indicate that essential oil of
thymus capitatus act as mixed-type inhibitor. According to
Ferreira and others (Bartos and Hackerman, 2000; Ferreira et
al., 2004), if the displacement in Ecorr values (i) >85 mV
ininhibited system with respect to uninhibited, the inhibitor
could be recognized as cathodic or anodic type and (ii) if
displacement in Ecorr is <85 mV, it could be recognized as
mixed-type. For studied inhibitor, the maximum displacement
range was 12 mV, which indicates that thymus capitatus oil is
mixed type inhibitor. It is clear from the results that the
addition of thymus capitatus oil caused a decrease in the
current density. The values of the corrosion current (Icorr) of
steel in the inhibited solution were smaller than this for
uninhibited solution. The parallel anodic Tafel plots obtained
in Figure 2 indicates that the hydrogen evolution is activation
controlled and the reduction mechanism is not affected by the
Table 1. Chemical constituents of Thymus Capitatus oil (%)
Composés Ir /lit Ir /apol Ir /pol %
α-Thujene 932 922 1031 0,6
-pinene 936 930 1029 2,9
Camphene 950 943 1070 3,2
1-octen-3ol 962 961 1449 1,2
Sabinene 973 965 1125 0,5
-pinene 978 970 1114 1,2
Myrcene 987 981 1162 1,8
-terpinene 1013 1010 1181 0,6
p-Cymene 1015 1015 1272 18,9
Limonene 1025 1022 1203 1,1
1,8-Cineole 1024 1022 1208 1,0
-terpinene 1051 1050 1247 2,5
trans hydrate de Sabinène 1053 1054 1463 0,8
Linalol 1086 1085 1545 1,5
Camphre 1123 1122 1511 1,2
trans-pinocarveol 1126 1124 1648 0,7
Borneol 1150 1153 1631 10,2
Terpinen-4-ol 1164 1163 1597 0,9
-Terpineol 1176 1174 1688 0,6
Myrtenol 1178 1180 1781 0,4
1-Methyl-3-methoxy-4-isopropylbenzene1215 1217 1766 1,2
carvacryl methyl ether 1226 1227 1559 1,1
Bornyle acetate 1270 1270 1578 1,2
Thymol 1267 1273 2168 1,5
Carvacrol 1278 1285 2193 13,4
-terpenyle acetate 1335 1335 1670 2,6
geranyl acetate 1362 1365 1753 12,2
transcaryophyllene 1421 1418 1595 2,9
-selinene 1476 0,3
germacrene D-4-ol 1566 2035 0,5
caryophyllene oxide 1578 1570 1965 1,9
-bisabolol 1659 1669 2200 0,6
6871 International Journal of Development Research, Vol. 06, Issue, 02, pp.6867-6874, February, 2016
presence of inhibitors (Elmsellem et al., 2014; Elmsellem et
al., 2014). These results demonstrated that the hydrogen
evolution reaction was inhibited and that the inhibition
efficiency increased with inhibitor concentration. The
electrochemical parameter values given in Table 2 reveal that
inhibition efficiency increases with an increase of the
concentration of inhibitors. We remark that the corrosion
current densities were more significantly reduced in the
presence of thymus capitatus oil. The best efficiencie obtained
in the presence of the inhibitor studied is 68% at 5mL/L.
Electrochemical impedance spectroscopy measurements
The inhibiting properties of the tested inhibitor have also been
evaluated by the determination of the polarization resistance.
The inhibition efficiency (E%) was defined as follow:
Where, R°corr and Rcorr are the charge transfer resistance in
presence and in absence of inhibitor, respectively.
The corresponding polarization resistance (RP) values of steel
in 1 M HCl in the absence and presence of different
concentrations of the inhibitor are given in Table 3. The
corrosion behavior of steel in 1M hydrochloric acidic solution,
in the absence and presence of oil thymus capitatus, is also
investigated by the EIS at 308 K after 30 min of immersion.
The charge-transfer resistance (Rt) values are calculated from
the difference in impedance at lower and higher frequencies.
The double-layer capacitance (Cdl) and the frequency at which
the imaginary component of the impedance is maximal (-
Zmax) are found as represented in the equation:
CdI=1 / ω.Rt (3)
ω = max2 f (4)
Where fmax is the frequency, at which the imaginary
component of the impedance (Zim) is maximum and Rt is the
diameter of the loop. Impedance diagrams are obtained for
frequency range 100 kHz to 10 mHz at the open circuit
potential for steel in 1M HCl in the presence and absence of
Table 2. Electrochemical parameters of steel at various concentrations of thymus capitatus oil in
1M HCl and the correspondinginhibition efficiency
Inhibitor mL /L -Eco -E(mV/SCE) βa (mV) ‐βc (mV) Icorr (mA/cm²) IE%
HCl 389 110 362 0.69 -----
1.25 401 64 242 0.29 58
2.5 396 55 227 0.27 61
5 394 56 226 0.22 68
Table 3.Corrosion parameters obtained by impedance measurements for mild steel in HCL 1M at
various concentrations of oil thymus capitatus
Inhibitor(mL/L) Re (Ω.cm Rt (Ω.cm2
F max (HZ) Cdl (µF.cm2
HCl 1.9 49 63 119 ----
1.25 3.2 101 79 19 51.5
2.5 6.5 111 63 22 56
5 1.7 142 14 7 65.5
Table 4. Gravimetric results of mild steel in acid solutions 1M HCl at different concentration of thymus
capitatus oil (308 K, 6 h)
Concentration (mL/L) W (mg/cm2
h) E% Θ = E%/100
Blanc 0.50 - -
1.25 0.26 48 0.48
2.5 0.24 52 0.52
5 0.185 63 0.63
Table 5. Corrosion parameters for mild steel in HCL 1M in absence and presence of optimum concentration of the
inhibitor studied (thymus capitatus oil) at different temperatures
T (°K) WHCl(mg/cm2
313 1.65 0.51 69
323 3.24 0.98 69
333 5.40 1.77 67
343 11.02 3.55 67
Table 6. Activation parameters Ea, ΔHa and ΔSa for the mild steel dissolution in 1M HCl in the absence and the
presence of oil thymus capitatus at optimum concentration (5 mL/L)
Inhibitor Ea (KJ/mol) ΔHa (KJ/mol) ΔSa (J/mol.K)
1M HCL 55.24 157.3 -197.02
Thymus capitatus Oil 48 172.1 -197.01
6872 El Ouadi et al. The use of essential oil of Thymus capitatus originating from North-East Morocco, as eco-friendly corrosion inhibitors
of mild steel in hydrochloric acid solution
Nyquist plots for steel in 1M HCl at different concentrations
presented in Figure 3. Table 3 gives values of charge-transfer
resistance Rt,double-layer capacitance Cdl, and fmax derived
from Nyquist plots and inhibition efficiency. As we notice, the
impedance diagrams show perfect semi-circles whose size
increases with the concentration of the inhibitor indicating a
charge-transfer process mainly controlling the corrosion of
steel. Similar diagrams were described in the literature for the
electrode of iron and steel with and without inhibitor in 1M
HCl (Bentiss et al., 1999; Elachouri et al., 2001) (Bentiss et
al., 1999; Elachouri et al., 2001). From the impedance data,
the charge-transfer resistance (Rt) increases with the inhibitor
concentration. Also, the double-layer capacitance (Cdl)
decreases with increase in the concentration of the inhibitor.
Weight loss corrosion rates and inhibition efficiency
Gravimetric measurements of steel were investigated in 1M
HCl in the absence and the presence of various concentrations
of oil thymus capitatus at 6 h of immersion and 308 K. The
following equation was used to determine the inhibition
Where W and Winh are the corrosion rate of steel in 1M HCl in
the absence and the presence of inhibitor, respectively. Table 4
summarizes the gravimetric trends of the steel immersed in
aerated molar HCl in the absence and the presence of the
inhibitor at various concentrations.It is clear that the corrosion
rate decreases with the increase of concentration of thymus
capitatus oil and in turn the inhibition efficiency (E %)
increases to attain 63% at 5mL/L.
Effect of temperature
The corrosion rate of steel with temperature was studied in
molar HCl both in the absence and presence of inhibitor at a
maximal concentration (5 mL/L) in the temperature range
313–343 K using weight loss measurements, the
corresponding results are summarized in Table 5. The
corrosion rate is more increased with the rise of temperature
for uninhibited acid solution. The presence of inhibitor leads
to a decrease in the corrosion rate (Figure 4). At elevated
temperature, the inhibitory action of inhibitor is slightly
increased and become nearly steady (67%). The activation
kinetic parameters such as energy (Ea), enthalpy (ΔHa) and
entropy (ΔSa) may be evaluated from the effect of temperature
using Arrhenius law (Eq. (6)) and the alternative formulation
of Arrhenius equation (Eq. (7)):
Where W is the corrosion rate, R the gas constant, T the
absolute temperature, A the pre-exponential factor, h the
Plank's constant and N is Avogadro’s number. Figures 5, 5’
show the plots of ln(W) against 1/T. Straight lines are obtained
with a slope of (−ΔHa
/R) and an intercept of (ln R/Nh+ΔSa
/R) from which the values of ΔHa
(Table 6). Inspection of Table 6 showed that the value of Ea
determined in 1M HCl containing thymus capitatus oil
(48KJ/mol) is less than that for uninhibited solution (55.24KJ/
mol). The decrease in the apparent activation energy may be
interpreted as a plot of Ln (CR/T) versus 1/T.
The straight lines are obtained with a slope (∆Ha/R) and an
intercept of (Ln R/Nh +ΔSa /R) from which the values of the
values of ∆Ha and ∆Sa are calculated for oil thymus capitatus
analyzed and are given in Table 6.Inspection of these data
revealed that the thermodynamic parameter (∆Ha) for
dissolution reaction of steel in 1M HCl in the presence of oil
thymus capitatus (172.1 KJ/mol) high than that of in the
absence of inhibitor (157.3 KJ/mol).The positive sign of ∆Ha
reflect the endothermic nature of the steel dissolution process
suggesting that the dissolution of steel is slow in the presence
of inhibitor. Negative value of entropies (∆Sa) imply that the
activated complex in the rate determining step represents an
association rather than a dissociation step, meaning that a
decrease in disordering takes place on going from reactant to
the activated complex.
In this paper, we have studied the corrosion inhibition of
Thymus capitatus oil for mild steel in 1M HCl solution by
gravimetric method and electrochemical techniques. The
results obtained are in good agreement and are given as
The analysis of essential oil isolated from Thymus
capitatus plant shows that its composition is dominated by
p-Cymene, carvacrol, geranyl acetate, borneol (18.9%,
13.4%, 12.2% and 10.2%, respectively).
Thymus capitatus oil act as mixed-type inhibitors without
modifying the mechanism of hydrogen evolution.
The adsorption onto the carbon steel surface was
characterized by the decrease in the cathodic and anodic
current densities observed in the potentiodynamic
polarization curves carried out in the presence of Thymus
The inhibition efficiency of Thymus capitatus oil increases
with the increase of inhibition concentration to reach 63%
The data obtained from the three different methods:
potentiodynamic polarization, EIS and weight loss have the
The inhibition efficiency of Thymus capitatus oil increases
slightly with the rise of temperature.
Thymus capitatus oil being natural and environmentally
benign products, they can be used as an alternative for
toxic chemical inhibitors in acidization and acid pickling of
Adams, R.P. 2004. Allured Publishing: Carol Stream.
Aouniti, A., Elmsellem, H., Tighadouini, S., Elazzouzi, M.,
Radi, S., Chetouani, A., Hammouti, B. and Zarrouk, A.
2015. Journal of Taibah University for Science,
Bartos, M. and Hackerman, N. 2000. J ElectrochemSoc, 139,
6873 International Journal of Development Research, Vol. 06, Issue, 02, pp.6867-6874, February, 2016
Belfilali, I., Chetouani, A., Hammouti, B., Louhibi, S.,
Aouniti, A. and Al-Deyab, S.S. 2014. Research on
Chemical Intermediates. 40, 1069.
Bentiss, F., Lagrenee, M., Traisnel, M. and Hornez, J.C. 1999.
Corros Sci., 41, 789.
Chetouani, A., Daoudi, M., Hammouti, B., Ben Hadda, T.,
Benkaddour, M. 2006. Corrosion Science. 48, 2987.
El Mounsi, H., Elmsellem, A., Aouniti, H., Bendaha, M.,
Mimouni, T., Ben Hadda, H.Steli, M., Elazzouzi, Y., EL
Ouadi and Hammouti, B. 2015. Anti-corrosive properties
of Nigella sativa L extract on mild steel in molarHCl
solution. Der PharmaChemica, 7(6):64-70.
EL Ouadi, Y., Bouratoua, A., Bouyanzer, A., Kabouche, Z.,
Touzani, R., EL Msellem, H., Hammouti1, B. and
Chetouani, A. 2015. Effect of Athamantasiculaoil on
inhibition of mild steel corrosion in 1M HCl. Der
El ouadi, Y., Bouyanzer, A., Majidi, L., Paolini, J., Desjobert,
J. M., Costa, J. Chetouani, A. and Hammouti, B. 2014.
Salvia officinalisessential oil and the extract as green
corrosion inhibitor of mild steel in hydrochloric acid. J.
Chem. Pharm. Res., 6(7):1401-141.
El Ouadi, Y., Bouyanzer, A., Majidi, L., Paolini, J., Desjobert,
J.M., Costa, J., Chetouani, A., Hammouti, B., Jodeh, S.,
Warad, I., Mabkhot, Y. and Ben Hadda, T. Evaluation of
Pelargonium extract and oil aseco-friendly corrosion
inhibitor for steel in acidicchloride solutions and
pharmacological properties. Res ChemIntermed. DOI
El Ouadi, Y., Lahhit, N., Bouyanzer, A., Majidi, L.,
Elmsellem, H., Cherrak, K., Elyoussfi, A. Hammouti, B.
and Costa, J. Chemical Composition and Inhibitory Effect
of Essential Oil of Lavande (Lavandula Dentata) LD on
the Corrosion of Mild Steel in Hydrochloric Acid (1M).
Arabian Journal of Chemical and Environmental
Research. Vol.1 N°2 (2015) 49–65.
Elachouri, M., Infante, M.R., Izquerdo, F., Kertit, S.,
Gouttaya, H.M. and Nciri, B. 2001. Corros Sci., 43, 19.
Elmsellem, H., Karrouchi, K., Aouniti, A., Hammouti, B.,
Radi, S., Taoufik, J., Ansar, M., Dahmani, M., Steli, H.
and El Mahi, B. 2015. Der Pharma Chemica, 7(10) 237-
Elmsellem, H., Aouniti, A., Khoutoul, M., Chetouani, A.,
Hammouti, B., Benchat, N., Touzani, R., Elazzouzi, M.
2014. Journal of Chemical and Pharmaceutical Research.
Elmsellem, H., Aouniti, A., Toubi, Y., Steli, H., Elazzouzi,
M., Radi, S., Elmahi, B., El Ouadi, Y., Chetouani, A. and
Hammouti, B. 2015. Der Pharma Chemica, 7 353-364.
Elmsellem, H., Aouniti, A., Youssoufi, M.H., Bendaha, H.,
Ben hadda, T., Chetouani, A., Warad, I. and Hammouti,
B. 2013. Phys. Chem. News. 70 84.
Elmsellem, H., Basbas, N., Chetouani, A., Aouniti, A., Radi,
S., Messali, M. and Hammouti, B. 2014. Portugaliae.
Electrochimica. Acta. 2, 77.
Elmsellem, H., Bendaha, H., Aouniti, A., Chetouani, A.,
Mimouni, M. and Bouyanzer, A. 2014. Mor. J. Chem., 2
Elmsellem, H., Elyoussfi, A., Sebbar, N. K., Dafali, A.,
Cherrak, K., Steli, H., Essassi, E. M., Aouniti, A. and
Hammouti, B. Maghr. J. 2015. Pure & Appl. Sci., 1 1-10
Elmsellem, H., Elyoussfi, A., Steli, H., Sebbar, N. K., Essassi,
E. M., Dahmani, M., El Ouadi, Y., Aouniti, A., El Mahi,
B. and Hammouti, B. 2016. Der Pharma Chemica, 8(1)
Elmsellem, H., Harit, T., Aouniti, A., Malek, F., Riahi, A.,
Chetouani, A. and Hammouti, B. 2015. Protection of
Metals and Physical Chemistry of Surfaces. 51(5) 873–
Elmsellem, H., Nacer, H., Halaimia, F., Aouniti, A., Lakehal,
I., Chetouani, A., Al-Deyab, S. S. Warad, I., Touzani, R.
and Hammouti, B. 2014. Int. J. Electrochem. Sci., 9, 5328.
Elmsellem, H., Youssouf, M. H., Aouniti, A., Ben Hadd, T.
Chetouani, A., Hammouti, B. 2014. Russian, Journal of
Applied Chemistry. 87(6) 744−753.
Ferreira, E.S. Giancomelli, C., Giacomelli, F.C. and Spinelli,
A. 2004. Mater. Chem. Phys., 83, 129.
Hochmuth, D., Joulain, D. and König, W.A. 2001. Library of
Massfinder 2.1, University of Hamburg Institute of organic
chemistry Hamburg Germany.
Joulain, D. and König, W.A. 1998. The atlas of spectral data
of sesquiterpene hydrocarbons. EbVerlag, Hamburg.
Kharchouf S. et al. 2011. Arabian Journal of Chemistry,
Manssouri, M., El Ouadi, Y., Znini, M., Costa, J. Bouyanzer,
A., Desjobert, J.M. and Majidi, L. 2015. Adsorption
proprieties and inhibition of mild steel corrosion in HCl
solution by the essential oil from fruit of Moroccan
Ammodaucusleucotrichus. Mater. Environ. Sci. 6 (3) 631-
Singha, A.K. and Quraishi, M.A. 2010. The effect of some bis-
thiadiazole derivatives on the corrosion of mild steel in
hydrochloric acid, Corros. Sci. 52 1373–1385.
Xia, S., Qiua, M., Yua, L., Liua, F., Zhao, H. 2008. Molecular
dynamics and density functional theory study on
relationship between structure of imidazoline derivatives
and inhibition performance, Corros. Sci., 50 2021–2029.
Znini, M., Bouklah, M., Majidi, L., Kharchouf, S., Aouniti, A.,
Bouyanzer, B. and Hammouti, J. 2011. Costa, SS Al-
Deyab, Int.J. Electrochem. Sci., 6, 691-704.
6874 El Ouadi et al. The use of essential oil of Thymus capitatus originating from North-East Morocco, as eco-friendly corrosion inhibitors
of mild steel in hydrochloric acid solution